### A

### R

### T

### I

### G

### O

### T

### É

### C

### N

### I

### C

### O

### C

### I

### E

### N

### T

### Í

### F

### I

### C

### O

**Introduction**

Transport of gases and vapors in polymers is an important subject both from technological and scientific point of view. Applications include protective coatings, packing materials for food, and selective barriers for gas or liquid mixture. In the case of food packages, polymeric materials should exhibit an adequate CO2/O2 ratio (generally lower than 7)[1]. The

process of permeation involves dissolution of the gas in one
side of the membrane, diffusion of the gas through it and
release of the gas from the other side of the membrane. When
dealing with glassy polymers, it is important to note that
permeability characteristics depend on thermal history of the
polymer[2]_{. A conventional method for determining}

permeability and diffusion coefficients in polymers involves
the measurement of membrane weight gain versus time until
the final mass of equilibrium is reached[3]_{.}

Photoacoustic (PA) spectroscopy and related photothermal
techniques[4-6]_{ are well-established spectroscopic techniques.}

The PA technique, apart from providing direct optical
absorption spectra[7,8]_{, can also be used to perform depth profile}

analysis[7,9]_{, and characterization of thermal properties}[10,11]_{.}

In addition, there has been a substantial development of new,
versatile and competitive instrumentation and experimental
methodologies suitable for use in daily practice. Further details
on the photothermal wave phenomenon and its applications
can be found in the books by Rosencwaig[4]_{ and Almond}[6]

and in some of many published reviews on the subject[5,12,13]_{.}

Recently, photothermal techniques have been applied to
the determination of diffusion coefficients in biopolymers[14]_{.}

However, the complete validation of this new methodology

demands the characterization of diffusion coefficients of plastic films commercially employed, which has been achieved successfully using traditional gravimetric techniques. Regarding this, the aim of the present work is to demonstrate the potentiality of photothermal techniques in the plastic packages quality control studying the diffusion properties of commercial low density polyethylene (LDPE) packages, a widespread used material for wrapping food and vegetables in day-to-day life. In order to support the gas diffusion results, thermophysical properties and crystallinity degree of samples are also determined.

**Materials and Methods**

*Materials and Characterization*
*Materials and CharacterizationMaterials and Characterization*
*Materials and Characterization*
*Materials and Characterization*

LDPE samples used in this work were obtained from
commercial transparent packages with thickness of 40µm
manufactured through conventional extrusion process by
Elanlec Embalagens (Campos dos Goytacazes, RJ), using
low density polyethylene with melt flow index 7.5 g/10min
and density 0.919 g/cm3_{ supplied by Polietilenos União in}

the form of pellets.

*Sample Crystallinity*
*Sample CrystallinitySample Crystallinity*
*Sample Crystallinity*
*Sample Crystallinity*

Membrane crystallinity was determined from X-ray diffraction analysis. A Seifert-FPM model URD65 X-ray generator with a Ni filter to provide Cu Ka radiation (λ = 0.1542 nm) was used. Scans were recorded at a scan speed of 0.1º and an exposure time of 10s. The degree of crystallinity, Xc was obtained from the diffractogram

according to the following relationship:

**Polyethylene Food Packages**

**Luiz H. Poley, Ana P. L. Siqueira, Marcelo G. da Silva, Helion Vargas**

**Laboratório de Ciências Físicas, UENF**

**Rubén Sanchez**

**Laboratório de Materiais Avançados, UENF**

**Abstract: The present work discuss the applicability of photothermal techniques for determining diffusion coefficients of**
oxygen and carbon dioxide of commercial low-density polyethylene (LDPE). The methodology involves the monitoring
of diffused gas by a photoacoustic analyzer. Diffusion coefficients measured for CO_{2} and O_{2} were 2.77 x 10-8_{ cm}2_{/s and}
1.68 x 10-7_{ cm}2_{/s, respectively. To support the gas diffusion results, thermal properties were studied using photoacoustic}
spectroscopy and crystallinity was determined using X-ray diffraction. Values obtained for thermal diffusivity and specific
heat capacity were 1.65 x 10-3_{cm}2_{/s and 2.33 J.cm}-3_{K}-1_{, which are in good agreement with values available in the literature}
for pure LDPE and thus assure reliability of diffusion coefficients values.

**Keywords**:* Photoacoustic spectroscopy, LDPE, diffusion coefficients.*

*T*
*A*
*T*
*C*

*A*

*A*

*A*

*X*

### =

### (

### −

### )

(1)Where AT denotes the total area of the diffractogram and AA

denotes the area corresponding to the amorphous region.

*Thermal Analysis*
*Thermal Analysis*
*Thermal Analysis*
*Thermal Analysis*
*Thermal Analysis*

Thermal behaviour of the films was determined in a
Calorimeter model DSC- 2010 from TA instruments, using
Indium as calibration reference. Samples of 20mg were heated
from 223K to 473K at 8K min-1_{ in aluminum pans. The}

enthalpy of fusion was used to determine sample crystallinity using the following relation:

0

*H*

*H*

*X*

*C*

*f*

### ∆

### ∆

### =

_{(2)}

Where Xc is the crystalline fraction, ∆Hf is the enthalpy of

fusion measured by DSC and ∆H0 is the enthalpy of fusion

for 100% crystalline polymer.

*Thermal Diffusivity Measur*
*Thermal Diffusivity Measur*
*Thermal Diffusivity Measur*
*Thermal Diffusivity Measur*
*Thermal Diffusivity Measurementsementsementsementsements*

LDPE packages were cut in small pieces (1cm X 1cm). The
room temperature characterization of the samples thermal
properties was based upon the measurements of the thermal
diffusivity, α, and of the heat capacity, ρ*c*p, where ρ is the

material density and *cp* the specific heat at constant pressure

(heat capacity per unit volume). To complete the determination
of the sample thermal properties, knowing α and ρ*c*p, the sample

thermal conductivity, *k*, is readily obtained from the equation
*p*

*c*

*k*

### =

### αρ

(3)The thermal diffusivity can be accurately measured by the
PA technique. This technique looks directly at the heat generated
in a sample, due to a thermal relaxation process, following the
absorption of light. Among several experimental set-ups the open
photoacoustic cell (OPC) method was used here. It consists of
mounting the samples directly onto a cylindrical electret
microphone and using the front air chamber of the microphone
itself as the usual gas chamber of conventional photoacoustic
cell[4]_{. As a result of a periodic heating of the sample following}

the absorption of modulated light, the pressure in the microphone chamber oscillates at the chopping frequency yielding the photoacoustic signal. The experimental arrangement (Figure 1a) consisted of a 100 mW Ar laser (Omicron Model 543-AP) whose beam was modulated with a mechanical chopper (EG&G Model 650). The sample was placed directly above the opening of the microphone convering it. The signal from the microphone was connected to a lock-in amplifier (EG&G Model 5210) used to register both signal amplitude and phase.

For the present samples, the contribution to the PA signal from the thermoelastic bending is the dominant. This effect is essentially due to the temperature gradient created inside the sample along an axis perpendicular to the surface

exposed to the incident radiation [15]_{. Owing to the existence of}

this gradient, a differential thermal expansion along sample
thickness is generated. This effect induces a periodic bending
of the sample in this direction (drum effect), *i.e.*, the vibrating
sample acts as a mechanical piston, producing the PA signal.
According to the theoretical development proposed by Rousset

*et al.*[15]_{, in the thermally thick regime (sample thickness }* _{l}*
s

exceeds the thermal diffusion length *m=(a/pf)* 1/2_{, where }_{f}_{ is}

the modulation frequency of the incident light), the pressure fluctuation in air chamber of the PA cell resulting from the thermoelastic displacement of the sample is proportional to

+ + + −

∝ ω π φ

δ 2 exp 1 1 1

1 1/2

2 *j* *t*

*x*
*x*
*f*

*p* (4)

where *x = l*s*a*s = *l*s(π*f*/αs)1/2 and tanφ = 1/(*x*-1). Eq. 3 means

that the thermoelastic contribution, at high modulation
frequency such that *x* >> 1, varies as *f*-1_{ and its phase πφ as}

###

###

###

###

###

###

### −

### +

### =

### 1

### 1

### arctan

*x*

*o*

### φ

### φ

_{ (5)}

Thus, for a thermally thick sample, if the thermoelastic contribution is dominant, the thermal diffusivity can be

evaluated from the modulation-frequency dependence of the signal amplitude, Eq.4, or its phase, Eq.5. In the derivation of Eqs. 4 and 5, Rousset and co-workers have assumed that the sample is optically opaque and that the heat flux into the surrounding air is negligible. The implicit optical opaqueness condition was ensured by the use of a thin circular absorbing Al foil (14 µm thick and 5 mm diameter) attached to the front surface of the sample using a thin layer of thermal paste to guarantee a good thermal contact between the sample and the Al foil. The thermal diffusion time in this Al foil is in the order of 13.6 ms so that the heat generated in the thin Al absorber is instantaneously transmitted to the sample.

*Heat capacity measur*
*Heat capacity measurHeat capacity measur*
*Heat capacity measurHeat capacity measurementementementementement*

The heat capacity per unit of volume, ρ*c*p, was measured

using the temperature rise method under continuous white
light illumination. Samples were painted on both surfaces with
a very thin film of black paint and were adiabatically
suspended in a Dewar flask, which was subsequently
vacuum-sealed (~10-2_{ Torr) (Figure 1b). Under these conditions the}

main heat-loss mechanism was by radiation. The Dewar flask has an entrance glass window through which the continuous white-light beam was focused onto one of sample surfaces. A thermocouple was attached on the opposite surface using thermal paste. In this way, the temperature evolution of the back surface could be monitored as a function of time. The surface temperature rise is given by[16]

### (

_{τ}

_{ρ}

### )

## (

/τ## )

0 *ls* *cp* 1 *e* *t*
*I*

*T* = − −

∆ (6)

where *I*0 is the intensity of the incident light and τ =* l*sρ*c*p/(2*H*)

is the rise temperature, *H* = 4σ*T*03 being the radiative

heat-transfer coefficient, where σ is Stefan-Boltzmann constant and

*T*0 is the ambient temperature. The parameter τ is determined

by fitting the exponential data with Eq. 6.

*Diffusion coefficient measur*
*Diffusion coefficient measurDiffusion coefficient measur*
*Diffusion coefficient measurDiffusion coefficient measurementsementsementsementsements*

Permeation studies of CO2 and O2 were performed using a

sample holder having its sides sealed off one from another. The permeate gas in study was introduced on one side and

kept at a constant pressure of 0.05 atm. On the other side the
concentration of the gas was measured using a photoacoustic
gas analyzer (URAS 14 from Hartman and Braun) as it was
being stored (Figure 2). The gas concentration rise, in these
conditions, is given by[14]_{:}

### )

### 1

### (

/0

*D*

*t*

*e*

*C*

*C*

### =

### −

− τ (7)Where C0 = gas concentration at saturation, τ*D*= *ls*2/2*D* = gas

diffusion time, where *D* is the gas diffusion coefficient and *ls*

is the sample thickness (40µm) in this case. Thus, by monitoring the time evolution of the gas concentration the gas diffusion time, τD, can be determined and thus, the

diffusion coefficient *D*. All measurements were performed
in room temperature (27 °C).

**Results and Discussion**

*Material Characterization*
*Material CharacterizationMaterial Characterization*
*Material CharacterizationMaterial Characterization*

In the X-ray diffractogram of LDPE (Figure 3), charac-teristics peaks can be identified at 21.5 and 23.8 of 2θ. Sample crystallinity degree obtained from X-ray diffractogram using eq. 1 was 38% .

From thermal analysis (Figure 4), glass transition temperature, melting temperature and heat of fusion of samples were determined as – 48 °C, 113 °C and 114 J/g,

**Figure 2.** Experimental arrangement used for gas diffusion studies.

**Figure 3.** X-ray diffractogram of LDPE.

respectively. Using the DSC enthalpy of fusion and taking
290J/g [17]_{ as the value for the fully crystalline LDPE, a value}

of 40% of crystallinity was found, in agreement with X-ray diffraction.

In Figure 5 is shown a typical PA signal frequency
dependence for low density polyethylene. It can be seen that
for modulation frequencies higher than 100 Hz, the signal
amplitude scales essentially as *f* -0.94,_{ a value close to }* _{f}* -1

_{.}

This frequency dependence of the PA signal of a thermally
thick sample confirms the thermoelastic bending as the
dominant mechanism responsible for the acoustic signal[18]_{.}

Accordingly, the thermal diffusivity was evaluated fitting
phase data to Eq. 5. Figure 6 shows experimental data and
fitting curve (solid line). The value of the thermal diffusivity
obtained from the data fitting was 1.65 x 10-3_{ cm}2_{s}-1_{, with an}

error of 5%. This value agrees with values present in literature
for pure LDPE[19]_{.}

To complete the determination of the thermal properties of the sample, we have measured the heat capacity per unit of volume. In Figure 7 is shown the back surface temperature arise as function of the time, after commencement of the sample illumination. The error in the data fit is about 10%.

Figure 7 also shows the cooling of the back surface of the
sample when the illumination is switched off. The solid lines
represent the best fit of the experimental data to Eq. 6 using τ
as an adjustable parameter. From the value of τ we obtained
the experimental value of the thermal capacity, ρ*c*p. We found

ρ*c*p= 2.33 J.cm-3K-1, with an error of 10%, for the LDPE

sample. The thermal conductivity *k* was determined using
the measured values of ρ*c*p and thermal diffusivity, *a* using

Eq. 3. The value obtained is 3.84 10-3_{ J.cm}-1_{K}-1_{s}-1_{, which is}

also in good agreement with values present in the literature[20]_{.}

*Diffusion Coefficients*
*Diffusion Coefficients*
*Diffusion Coefficients*
*Diffusion Coefficients*
*Diffusion Coefficients*

Concentrations of CO2 and O2 in the analyzer chamber in

function of time are presented in Figure 8. The fitting of experimental data to Eq. 7 allows the determination of diffusion coefficients. The values obtained for diffusion coefficients of LDPE to O2 and CO2 were 1.68 x 10-7 cm2/s and 2.77 x

10-8_{ cm}2_{/s, respectively. These values agree with those}

presented in literature for LDPE [20]_{(6.9 x 10}-8_{ cm}2_{/s for CO}
2

and 4,6 x 10-7_{ cm}2_{/s for O}

2). Differences can be probably

**Figure 5.** Modulation frequency dependence of PA signal for LDPE.

**Figure 6.** Dependence of PA signal phase on the chopping frequency for
LDPE.

**Figure 7.** Back surface temperature evolution for LDPE during heating (a)
and cooling (b). The solid line represents the best fit of the experimental
data to Eq.6 using τ as an adjustable parameter.

attributed to differences in the thermal history of the material,
since it causes variations in crystallinity degree and
morphology. These features may introduce a sensitive impact
in the barrier effect in the polymer, since crystallites are
considered to be impermeable and morphology affects
segmental chain mobility in amorphous phase, which plays
important role in diffusion[21,22]_{. This explanation can be}

supported by experimental results obtained using conventional
techniques that point out a decrease of 80% in permeability of
polyethylene to nitrogen, carbon dioxide and oxygen in
consequence of a variation of 20% in sample crystallinity[23]_{.}

Considering this, it can be said that the photothermal method for determining diffusion coefficients in polymers gives reliable results which enlarges its horizons in the characterization of materials.

**Conclusion**

In this paper we have reported on the measurements of the thermal and sorption properties of Low-density Poly-ethylene packages using the PA techniques. The results agree with values available in literature using conventional techniques, which indicates the success of the methodology used.

**Acknowledgments**

The authors wish to thanks CAPES and CNPq for the financial support to this work.

**References**

1. Marais, S.; Saiter J. M.; Devallencourt, C.; Nguyen, Q.T.; Métayer, M. – Polymer Testing 21 p. 425, (2002).

2. Compañ, V.; Ribes, A.; Díaz-Calleja, R.; Riande, E. – Polymer 37 p. 2243, (1998).

3. Neogi, P. *- Diffusion in Polymers*; Marcel Dekker, New
York, (1996)

4. Rosencwaig, A. *- Photoacoustic and Photoacoustic*
*Spectroscopy*; Wiley; New York, (1980).

5. Vargas, H. and Miranda, L. C. M. - Phys. Rep. 161 p.43, (1998).

6. Almond, D. and Patel, P. *- Photoacoustic and Photothermal*
*Science and Techniques*; Chapman and Hall; London,
(1966).

7. Nery, J. W.; Pessoa Jr, O.; Vargas, H.; Reis, F. A. M.; Vinha, C.; Gabrielli, A. and Miranda, L. C. M. - Analyst 112 p.1487, (1987).

8. Anjo, A. M. and Moore, T. A. - Photobiology 39 p.635, (1984).

9. Busse, G. - Appl. Opt. 31 p.107, (1982).

10. Alvarado-Gil, J. J., Vargas, H.; Sanches-Sinencio, F.; Gonzales-Hernadez, J and Miranda, L. C. M. - Opt. Eng. 36, p.348, (1997).

11. Calderon, A.; Alvarado-Gil, J. J.; Gurevich, Y. G.; Cruz-Orea, A; Delgadillo, I., Vargas, H. and Miranda, L. C. M. - Phys. Rev. Lett. 25, p.5022, (1997).

12. Kinney, J. B. and Staley, R. H. - Annu. Rev. Mater. Sci. 12, p.295, (1992).

13. Torres-Filho, A.; Leite, N. F.; Miranda, L. C. M.; Cella, N.; and Vargas, H. - J. Appl. Phys. 66 p. 97, (1989).

14. Silva, M. G.; Gonçalves, S. S.; Sthel, M. S.; Schramm, D. U.; Sánchez, R. R.; Rieumont, J. B.; Vargas, H. – Rev Sci Instrum 74, p. 831, (2003).

15. Rousset, G.; Lepoutre, F. and Bertrand, L. - J. Appl. Phys. 54 p.2383, (1983).

16. Hatta I. *- Rev. Sci. Instrum.*, *50*, 292, (1979).

17. Wunderlich, B. *- Thermal Analysis*; Academic Press, New
York, (1990).

18. Leite, N. F.; Cella, N.; Vargas, H. and Miranda, L. C. M. - J. Appl. Phys. 61 p.3025, (1987).

19. Grzegorczyk, D.; Feineman, G. - Handbook of Plastics in Eletronics, Reston, (1974).

20. Brandup, J.; Immergut, E. H. *- Polymer Handbook,* John
Wiley & Sons, New York, (1989).

21. Aniello, C.; Guadagno, L.; Gorrasi, G. and Vittoria, V. – Polymer 41 p.2515, (2000).

22. Hedenqvist, M.; Gedde, U. W. – Prog. Poly. Sci. 21 p. 299, (1996).

23. Comyn, J. *- Polymer Permeability*; Elsevier, London,
(1985).